Dec 24, 2018 - Amongst contemporary semiconductors many of the best performing materials ... However, the race towards ever higher mobilities resulted in ...
s. â1 is obtained. Owing to the highly scalable crystalline film formation, the dip coating ... exhibit a high molecular disorder and a low degree of crystallinity,.
Publication Date (Web): April 2, 2018 ... The dependence of the DMS behavior on the position of the carbonâcarbon double bond within the ionized lipid is ...
6 days ago - importance of direct, through-space interactions between the charge site and the carbonâ carbon double ..... Free energy landscape for the [M + H]+ ions of 1-deoxySO (n-x, trans) isomers (where x = 4, 5, 6, 10, 13, and 14) based on DFT
Formation and Evaluation of Derivatives, Preparation and Insecticidal Evaluation of ... Insecticidal evaluation of two unsaturated alcoholic derivatives of a ...
Nov 29, 2007 - Recently, we developed several high-performance, air-stable, molecular semiconductors for vacuum-processed OFETs.5 In the course of our studies, we found that benzothieno[3,2-b]benzothiophene (BTBT) is a promising core structure
Thin films of the organic semiconductors deposited on Si/SiO2 substrates by spin coating have well-ordered structures as confirmed by XRD analysis. Evaluations of the devices under ambient conditions showed typical p-channel FET responses with the fi
... [3H]GR 113808, a 5-HT4 receptor selective ligand, in the rat striatum and the electrically stimulated myenteric plexus longitudinal muscle of the guinea pig.
The improved stability is extremely valuable for realizing long-lived organic electronic devices. In summary, high-performance oligofluorene derivatives have ...
Sep 1, 1995 - Universita di Padova, 35100 Padova, Italy, and MRC Collaborative Centre, Mill Hill, London NW7 lAD, U.K.. Received February 2, [email protected]
Subscriber access provided by University of South Dakota
Organic Electronic Devices
Mobility Evaluation of BTBT Derivatives: Limitation and Impact on Charge Transport Robert Wawrzinek, Jan Sobus, Mujeeb Ullah Chaudhry, Viqar Ahmad, Arnaud Grosjean, Jack K. Clegg, Ebinazar B. Namdas, and Shih-Chun Lo ACS Appl. Mater. Interfaces, Just Accepted Manuscript • DOI: 10.1021/acsami.8b16158 • Publication Date (Web): 24 Dec 2018 Downloaded from http://pubs.acs.org on December 25, 2018
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Mobility Evaluation of BTBT Derivatives: Limitation and Impact on Charge Transport Robert Wawrzinek,a,b,† Jan Sobus,a,b,† Mujeeb Ullah Chaudhry, a,b Viqar Ahmad,a,b Arnaud Grosjean,c Jack K. Clegg,c Ebinazar B. Namdasa,b,* and Shih-Chun Loa,c,* a
Centre for Organic Photonics & Electronics, The University of Queensland, Brisbane, Queensland 4072, Australia b School of Mathematics and Physics, The University of Queensland, Brisbane, Queensland 4072, Australia. c School of Chemistry and Molecular Biosciences, The University of Queensland, Brisbane, Queensland 4072, Australia. *Correspondence
ABSTRACT Amongst contemporary semiconductors many of the best performing materials are based on benzothieno[3,2-b]benzothiophene (BTBT). Alkylated derivatives of these small molecules not only provide high hole mobilities but can also be easily processed by thermal vacuum or solution deposition methods. Over the last decade numerous publications have been investigating molecular structures and charge transport properties to elucidate what makes these molecules so special. However, the race towards ever higher mobilities resulted in significantly deviating values, which exacerbates linking molecular structure to electronic properties. Moreover, a recently arisen debate on overestimation of organic field-effect transistor mobilities calls for a revaluation of these numbers. We synthesised and characterised four BTBT derivatives with either one or two alkyl chains (themselves consisting of either 1 ACS Paragon Plus Environment
eight or ten carbon atoms), and investigated their spectroscopic, structural and electrical properties. By employing two probes, gated 4-point probe and gated van der Pauw measurements, we compare field effect mobility values at room and low temperatures, and discuss their feasibility and viability. We attribute mobility changes to different angles between molecule planes and core-to-core double layer stacking of asymmetric BTBT derivatives and show higher mobilities in the presence of more and longer alkyl chains. A so called “zipper effect” brings BTBT cores in closer proximity promoting stronger intermolecular orbital coupling and hence higher charge transport.
INTRODUCTION Semiconducting thienoacenes were first applied in organic field-effector transistors (OFETs) in the 1990s, albeit showing only moderate hole mobilities. In the mid-2000s, the first molecules based on benzothieno[3,2-b]benzothiophenes (BTBT) gave unprecedented high mobilities of up to 2.0 cm2/Vs, leading to an increasing interest in these structures ever since.1 To date, the literature provides a plethora of examples of BTBT derivatives used as hole transport layers in OFETs, photo-transistors and organic light-emitting transistors (OLETs). 2-6 Over the years, alkylated variants turned out to provide superior performances, with C8-BTBTC8 as their most prominent representative.
As solution and vacuum deposition are feasible fabrication techniques, record-high mobilities of up to 50 cm2/Vs have been reported (a comprehensive selection of BTBT semiconductors and their reported OFET performances can be found in Table S1 in the Supporting Information). However, it was just recently that a reconsideration regarding the determination of OFET charge mobility has caused many doubts in how to interpret values from different sources and how to derive structure-property relations from them. 7-9
Transistor mobility calculation by conventional current-voltage equations strongly depends on device geometry and does not account for contact resistance caused by the presence of an injection barrier. The latter arises from an energetic mismatch between the charge injecting metal electrode and the organic semiconductor’s energy level (i.e., the highest occupied molecular orbital for p-channel transistors). Furthermore, polycrystalline films generally exhibit a high degree of disorder, evoked by varied chain length and angles, defects, voids and crystal boundaries. These factors in turn provoke inhomogeneous carrier mobilities at different carrier concentrations impeding reliable mobility calculations from simplistic MOSFET 3 ACS Paragon Plus Environment
current-voltage equations. Often, but not necessarily, overestimated mobilities were derived from current against voltage plotted measurements showing a “kink” between linear and saturation regime.9 A recent review provides in depth analysis of the impact of contact resistance and importance of protocols used for mobility extraction.10 Gated 4-probe measurements eliminate the issue of contact resistance but are geometry dependent. 11,12 Also correct probe positioning and confinement of the organic layer are crucial to generate meaningful results and avoid overestimation.7,13 A third approach to mobility calculation is the gated van der Pauw method, which removes both of the above limiting factors (i.e., geometry factor and contact resistance) and allows for feasible performance statistics, since a single device can be measured in eight different orientations.
In this article, we aim to provide a contemporary experimental comparison between the three above mentioned methods in the context of alkylated BTBT semiconductors. A recent theoretical study identified the restraining forces of longer alkyl chains (Cn > 8) to promote a herringbone arrangement, as compared to the - stacking of BTBT derivatives with shorter chains. The resulting increase in molecular order enables a strong/balanced intermolecular charge-transfer, as well as reduced electron-phonon coupling and consequently in high mobility BTBT semiconductors.14 Thus, we selected a set of molecules that form herringbone structures varying in two parameters – number of surface groups and length thereof. Those five molecules are shown in Figure 1 and include the widely used and commercially available C8BTBT-C8 as well as the parental BTBT as a benchmark. All molecules were synthesised, fully characterised and investigated under identical conditions (details are provided in the Supporting Information). We present structural and electronic properties based on crystal structures, XRD, AFM and the aforementioned mobility measurements at room and low temperatures, reaching 70 K. Mobilities are then discussed concerning reliable value extraction, 4 ACS Paragon Plus Environment
impact on charge transport mechanisms as well as structure property relationships of BTBT derivatives.
Figure 1. Molecular structures of parental, mono- and di-alkylated BTBTs (all alkyl chains are linear). RESULTS AND DISCUSSION Material synthesis: All BTBTs reported here were synthesised following literature procedures.15-18 Detailed experimental procedures and characterization are described in the Supporting Information.
Spectroscopic properties of alkylated BTBT derivatives Absorption and photoluminescence spectroscopy in toluene of the mono- and di-alkylated BTBT in this study show almost identical spectra, suggesting a marginal influence of the alkysubstitution on the chromophore (Figure S1A and S1B in Supporting Information). As expected, the length of the alkyl chains also does not affect the solution spectroscopic properties. However, when investigating evaporated thin films on quartz glass, the unique supramolecular order in BTBTs becomes evident and differences appear (Figure S1C): The solid state absorption spectra bathochromically shift with increasing number and length of the alkyl chain attached. It is also due to these long-range structures that accurate energetic 5 ACS Paragon Plus Environment
information on BTBTs (e.g., ionization potentials, IPs) need to be derived from solid state rather than solution measurements.19 The photoluminescence spectra on the other hand seem to be less affected by those factors (Figure S1D).
Structural properties of alkylated BTBT derivatives Figure 2 shows crystal structures of all BTBT derivatives. As mentioned before, the supramolecular order of BTBTs in solid state causes significant changes in the materials’ properties when compared to those in solution. These long-range structures also massively contribute to charge transport in OFETs, hence, examination of crystal structures can help to gain insight in packing parameters that facilitate high transistor performance. Most fused thiophene containing semiconductors exhibit a herringbone packing, where side-by-side S∙∙∙S(C) interactions overrule CH∙∙∙ interaction of the aromatic rings, which otherwise would lead to a face-to-face orientation. The BTBT derivatives of this study are no exception and each molecule is surrounded by four edge-on and two off-set adjacent neighbours (Figure 2). This orientation can be enforced or disturbed by addition of surface groups. For instance, Ruzié et al. showed that alkoxy groups cause an offset between adjacent BTBT cores resulting in poor hole mobilities when employed in OFETs.19 Introduction of such functional moieties can polarise the chromophore’s electron distribution. This increases π-π electronic repulsion, hence, forcing the molecules into a slipped-stacked packing.20
Figure 2. Herringbone packing of BTBTs (crystal structures of BTBT, BTBT-C8, C8-BTBTC8 and C10-BTBT-C10 were obtained from the literature.). 21-23 ds is the intermolecular distance between adjacent sulphur atoms that show relevant angles for potential orbital overlap, dc is the distances between the four edge-on BTBT core centroids of each molecule and is the Herringbone angle between molecule planes. Additionally to the edge-on packing observed in the parental BTBT, alkylated derivatives reduce the distance to their molecular neighbours due to the so called “zipper/fastener effect” induced by attractive dispersion forces.17,24,25 Minemawari et al. calculated higher interaction energies for increased alkyl-substituted BTBTs.26 Alkan and Yavuz calculated that shorter alkyl chains in Cn-BTBTs-Cn (n = 3–5) exhibit strong -stacking arrangements which tends to lean to a band-like transport. On the other hand, longer alkyl chains (n = 8, 10, 12) cause a herringbone arrangement, which can be better described by a hopping model. 14 Interestingly, 7 ACS Paragon Plus Environment
when comparing distances between the four edge-on BTBT core centroids of each molecule (dC Figure 2 inset), no general trend is observed. The proposed narrowing of the Herringbone angle is only apparent within the mono- or di-alkylated groups. However, the zipper effect brings sulphur atoms of edge-on neighbours in such close proximity that intermolecular orbital coupling is enabled.1 This unique arrangement provides an unusual path for charges through the thin film – unlike most organic semiconductors, BTBT’s charge transport seems to take place perpendicular to the chromophores’ conjugated π-system. 25 It was suggested that the balance of - and tilted packing in BTBT molecules with herringbone arrangements is beneficial for charge transport. 14 When calculating the intermolecular distance between adjacent sulphur atoms that show relevant angles for potential orbital overlap (dS in Figure 2 inset), it becomes apparent that this value decreases with number and length of the alkyl chains. It is noted that this average distance of the parental BTBT (0.399 nm) is smaller than in case of BTBT-C8 (0.412 nm). Analysis of the X-ray diffraction (XRD) patterns of evaporated films (Figure S2A) provides more insight: Symmetric BTBT derivatives show main diffraction peaks that can be directly attributed to stacking molecule layers, with a calculated spacing close to the theoretical length of the molecule (Figure S2B, Table S3). Smaller peaks at higher angles appear at the integer multiplications of the main peak, showing higher orders of diffraction. However, for asymmetric BTBTs, the two tallest peaks appear at the spacing corresponding to single and double molecule length, indicating core-core double-layer stacking (as presented in Figure 2). Peaks of higher order appear as well but, as opposed to the doubly alkylated molecules, less pronounced. These results are supported by AFM images (Figure S3 in the Supporting Information): For all compounds a layered, terrace-like structure is observed. While for the symmetric molecules the step height directly corresponds to the molecule length, in asymmetric BTBTs a step twice the molecule’s length is encountered much more frequently than the one corresponding to the single molecular layer. In addition, a longer alkyl chain (C 10 8 ACS Paragon Plus Environment
versus C8) promotes higher surface roughness in both cases (mono- and di-alkylated), especially pronounced in the case of BTBT-C10.
Mobility extraction: This section will compare conventional two-probe, gated four-probe and gated van der Pauw mobility measurements. For each of the four BTBT derivatives, three types of devices (Transistor Transmission Line - TTL, Gated Four Point Probe -gFPP, Gated Van Der Pauw gVDP) were prepared – the shared cross section can be seen in Figure 3A. All devices were manufactured on top of 0.5 mm thick Si wafer, acting as a substrate and gate electrode, covered with 400 nm of Si nitride acting as a dielectric layer. Additionally, a thin (~80 nm) polymethylmethacrylate (PMMA) layer was deposited on top of the nitride as a passivation layer, to minimize trapping at the dielectric-semiconductor interface. The total capacitance per unit area (CI) value was equal to 12 nF/cm2, which was calculated using PMMA thickness and dielectric constant and verified by LCR meter (Keysight E4980A). Next, 30 nm thick organic semiconductor layers were deposited using thermal evaporation through the shadow mask. They were followed by evaporation of contact electrodes consisting of 5 nm thick molybdenum oxide layer acting as a hole injecting layer and 35 nm gold layer. Shadow mask layouts (organic layer in red and contacts in blue) are presented in Figure 3B-D for TTL, gFPP and gVDP device architectures respectively. Thicknesses of the deposited layers were verified using DektakXT profilometer. Electrical characteristics were obtained using the Agilent B1500A semiconductor analyzer. Low temperature measurements were collected using the same device analyzer plugged to a Janis CCR12 cryogenic probe station cooled with Sumitomo HC-4E helium compressor system. The results of electrical measurements (exemplarily shown for C8BTBT-C8) are presented in Figure 3E–G. Results for the other BTBTs are provided in the Supporting Information. 9 ACS Paragon Plus Environment
Figure 3. Shadow mask design employed in this study and mobility characteristics obtained for C8-BTBT-C8 using three different techniques. Generalised cross-section of devices used in this study (A). Transistor transmission tine (TTL) (B), gated Four Point Probe (gFPP) Method (C), gated van der Pauw (gVDP) Method (D). Linear (lin) and saturation (sat) mobility extracted from Transistor Transmission Line measurements for various channel widths and increasing length (E); conductivity plot for the gated four-point probe device for driven at varying source-drain voltages with the extracted mobility in the inset (F); gated van der Pauw conductivity plot combining eight measurements under different orientations for a single device (G). Conventional two probe mobility measurements Traditionally, the mobility of the OFET is extracted from their electrical characteristics by employing equations commonly used for the inorganic MOSFET devices:
𝑉 −𝑉 − 𝑉
𝑉 𝑤ℎ𝑒𝑛 𝑉 < (𝑉 − 𝑉 ) − 𝑙𝑖𝑛𝑒𝑎𝑟 𝑟𝑒𝑔𝑖𝑚𝑒
(𝑉 − 𝑉 ) 𝑤ℎ𝑒𝑛 𝑉 > (𝑉 − 𝑉 ) − 𝑠𝑎𝑡𝑢𝑟𝑎𝑡𝑖𝑜𝑛 𝑟𝑒𝑔𝑖𝑚𝑒
Here, ISD is the source-drain current density, W is channel width, L is channel length, µ is the charge carrier mobility, CI is the capacitance per unit area, VD and VG are the bias voltages of the drain and gate electrodes respectively and the source electrode is grounded, VS = 0. While these equations do not take into account the subthreshold behaviour or electric field degradation of mobility (as more sophisticated models do).27 However, their results are still sufficient for a general evaluation of channel material performance. Usually, transfer characteristics ISD(VG) swipe at fixed VD - low VD for linear mobility, high VD for saturation mobility) are measured and then, based on equation (1), the mobility is extracted from the slope of ISD versus VG or √ISD versus VG for linear and saturation regimes, respectively. However, this approach has two fundamental flaws. First, it does not take into account the contact resistances present in the device (which come from the electrodes, electrode-material interface or even the vertical transport in the material itself), thus lowering the obtained mobility value. Second, the obtained mobility value strongly depends on the geometric factor L/W. Small variation in one or both of 11 ACS Paragon Plus Environment
those parameters (especially channel length L, which usually is in the range of tens of microns) can lead to significant error in the obtained mobility value. The nature of the contacts itself (Ohmic or Schottky type) and the resulting deviation from those ideal equations can lead to errors in several orders of magnitude, as has been described in detail elsewhere.9 Therefore, we describe in the following three measuring methods we employed in order to evaluate the BTBT derivatives, which mitigate one or both of these problems.
Transistor transmission line (TTL) method One of the ways of estimating the impact of the contact resistance is performing the series of mobility measurements on transistors with changing channel length L by keeping the channel width W constant (exemplarily shown in Figure 3E). Figure 3B shows three organic zones comprising of transistor widths of 0.5 mm, 1 mm and 1.5 mm (red colour) to create transistor transmission lines with channel lengths ranging from 80 µm to 400 µm (the blue colour indicates alternating electrodes). Typical transfer characteristics obtained from those devices are shown in the Supporting Information of Figure S5. Assuming the total resistance of the device being the sum of constant contact resistance and channel resistance varying with length (2), one can quickly derive that the extracted apparent mobility will be lower than the intrinsic mobility (3).7,28 This deviation will be particularly high for short channel length devices. With the increase of L, the measured mobility converges to the “true” value. Based on the series of measurements, both the contact resistance and true mobility can be estimated. 𝑅 𝜇
Where Rc and Rtot is contact and total resistance respectively. Although this method does not eliminate W and L dependence of the obtained results in terms of the absolute mobility value, 12 ACS Paragon Plus Environment
the number of devices produced on a single substrate provides a nice statistical picture. Detailed results for the remaining alkylated BTBTs can be seen in Figure S6A, S7A and S8A. As expected, the mobility from the TTL experiment increases with increasing channel length, both in linear and saturation regimes. The saturation mobility for C8-BTBT-C8 showed the highest (4.1 cm2/Vs) and BTBT-C8 the lowest mobility value (0.3 cm2/Vs). Interestingly, the longer alkyl chain of BTBT-C10 tends to give higher mobilities in both the linear and the saturation region. Also, di-alkylated BTBT derivatives yielded higher mobility than their single-sided counterparts.
Gated four-point probe (gFPP) method The four-point probe method for measuring conductivity was first used more than a century ago.11 By introducing two additional voltage probes between source and drain electrodes in the current channel, one can entirely eliminate the influence of contact resistance. It is no surprise that this technique was soon implemented for mobility measurements in field-effect devices as a Gated Four Point Probe method, where the mobility is given by (4). 𝜇
𝑤ℎ𝑒𝑟𝑒 𝜎 = |
Here, D is the distance between the voltage probes and VP1 and VP2 are their respective potentials. However, this method also has its drawbacks as it is even more prone to geometry errors and requires precise dimension values of all electrodes and distances between them. Moreover, when designing such an experiment, the L/W ratio should be kept as low as possible to avoid mobility overestimation. In order to prevent channel shunting, this also holds true for the width of the probes.29 Furthermore, the organic layer itself should be confined to the area between source and drain to avoid mobility overestimation.13 Based on those considerations, we designed the electrode arrangement shown in the inset of Figure 3C with four different devices on each substrate (W = 2500 µm, L = 400 µm; W = 2500 µm, L = 600 µm; W = 1500 13 ACS Paragon Plus Environment
µm, L = 400 µm; W = 1500 µm, L = 600 µm) and narrow (60 µm wide) voltage probes. Here, the red and blue colours represent the organic layer and the metal electrodes, respectively.
Figure 3F shows the sheet conductivity versus gate bias exemplarily for C8-BTBT-C8 with three different source-drain voltages ranging from -10 V to -20 V. One can observe slight hysteresis in the obtained curves (especially for lower VDS) and dips in mobility for very small and very large gate voltages. Yet, for the gate voltages ranging from -30 to -90 V, the mobility value remains stable and flat. Corresponding plots for the remaining BTBT derivatives can be found in the Supporting Information (Figures S6B, S7B and S8B). While the symmetric BTBTs show values well agreeing with the results from TTL measurements (mobility around 4 cm2/Vs), the plots obtained for the mono-alkylated BTBT derivatives deviate significantly from linearity and are therefore not reliable for determination of a single value of mobility. Even after deriving the mobility from the steepest slope of the plot, the values remain lower (around 1 cm2/Vs) than the ones for the di-alkylated counterparts.
Gated van der Pauw (gVDP) method Important generalization of the four point probe method for conductivity measurements have been proposed by van der Pauw in the 1950s.30,31 By using the appropriate “clover-like” shape of the organic layer, one can change the geometric factor L/W into a constant value of ln(2)/π. Moreover, the four-fold symmetry of the device allows eight different measurement orientations, which can detect any possible anisotropy (if present) in the sample, thus providing more data for averaged performance. Lately, a gated version of the van der Pauw method has been applied as a measuring tool for organic semiconductor layers with excellent results.32 The arrangement of electrodes used in this experiment is given in the inset of Figure 3D. Here, the red and blue colours represent the organic layer and the metallic electrodes, respectively. 14 ACS Paragon Plus Environment
During the measurement, a constant current flow is maintained between source and drain electrode (chosen as any pair of adjacent electrodes) by the source-drain bias. While the gate voltage is changed, source-drain bias changes accordingly to maintain the current. Source-drain bias and the biases on the two other electrodes acting as voltage probes VP1 and VP2 are monitored. This is exemplarily shown for C8-BTBT-C8 in Figure 3G, where differently coloured points correspond to eight different electrode/current flow orientations. No directional or geometric dependence in the obtained results was observed. Subsequently, the sheet conductivity can be calculated using equation (5), which leads to extraction of mobility values by (6). 𝐼
= 𝜎 |𝑉
𝐶 |𝑉 − 𝑉 − 𝑉 |𝑤ℎ𝑒𝑟𝑒𝑉 =
Here, ISD is the (constant) source-drain current, CI is the capacitance per unit area of the dielectric layer, VG is the applied gate potential, VT is threshold voltage and µtrue is the extracted mobility. The obtained mobility value should be constant with changing source-drain currents (Figure S4A). From the obtained characteristics, it is also possible to easily distinguish between the linear and saturation regime (Figure S4B). The extracted mobility for C8-BTBTC8 reaches up to 4.2 cm2/Vs, which is close to the value obtained by the other two methods (Figure 3E and 3F). Corresponding plots for the remaining BTBT derivatives can be found in the Supporting Information (Figures S6C, S7C and S8C). Owing to the elimination of both major problems connected with mobility measurements – geometry dependence and impact of contact resistance – we consider the gated van der Pauw method to be the most reliable for measurements of mobility in organic thin films.
The mobility values collected by the three methods are summarised in Table 1: It shows that doubly-alkylated BTBTs are in general performing better than their mono-alkylated counterparts and that molecules with a shorter (-C8) alkyl chain give more reproducible results. The first observation can be attributed to the core to core stacking in case of mono-alkylated molecules (as confirmed by XRD and AFM), which provides a “sideway” pathway for hole transport. In addition, BTBT-C8 exhibited a significantly larger herringbone angle and distance between molecules within a single plane than the other three compounds. This seems to be the defining factor behind its generally lower performance. The smaller dihedral angle of the BTBT-C10 enables higher mobility values, however, albeit having a quite low film quality (surface roughness of 12.6 nm). On the other hand, both bi-alkylated BTBTs show fairly consistent results with mobilities of similar magnitude. The slightly better result uniformity of C8-BTBT-C8 (when compared to C10-BTBT-C10) can be attributed to better film quality (low surface roughness of ~2 nm, less grainy surface with larger domains). Our results confirm that C8-BTBT-C8 is rightfully the BTBT derivative of choice in industry standards.
Table 1. Comparison of mobility values obtained for different BTBT derivatives using transistor transmission line (TTL), gated Four Point Probe (gFPP) and gated van der Pauw (gVDP) methods. (LIN = linear regime; SAT = saturation regime). Material
* gFPP values for mono-alkylated BTBT derivatives are most likely over-estimated due to the leakage current overwhelming the source-drain current for those samples (see Figures S7B and S8B in the Supporting Information). Understanding the charge transport mechanism – low temperature (T) measurements. 16 ACS Paragon Plus Environment
In order to understand the charge transport mechanism within the BTBT derivatives, we performed temperature dependent mobility measurements for gVDP devices (Figure 4).
Figure 4. Mobility values obtained from gVDP devices for different BTBT derivatives plotted as a function of inverse temperature. Dotted lines are added as guide to the eye indicating transition between two mobility regimes (steeper for better conducting compounds). It becomes apparent that the mobility’s temperature dependence in these devices does not follow an Arrhenius-like behaviour. Instead, there are two distinct mobility regions – a high T region where the mobility is strongly temperature dependent and a low T region where it is almost independent. Such behaviour has been previously observed in OFETs and explained as a result of several phenomena including metal-to-insulator transition, 33,34 Fowler-Nordheim tunneling35 or a Luttinger liquid transport model.36 As the curves from Figure 4 are similar in shape for all BTBT derivatives, we chose C8-BTBT-C8 as a model system to study the underlying transport mechanism in these compounds. First, we fabricated devices with three different thicknesses (10, 20, and 30 nm) of C8-BTBT-C8 to confirm that vertical charge transport from the electrode contact towards the conductive channel is not the limiting factor, as it has been shown for high-mobility epitaxial devices.37 From Figure S9 in the Supporting 17 ACS Paragon Plus Environment
Information, one can see that such thickness modifications virtually cause no difference in device performance.
Next, output characteristics for the 20 nm device were measured for temperatures ranging from 300 K down to around 80 K, enabling the three dimensional analysis (T, VSD, VG). We plotted the obtained channel conductivity as a function of T-1/2 for different gate and source drain biases (Figure 5). A transition between two conductivity regimes, similar to the situation in Figure 4, can be seen on these plots: At high VSD bias (corresponding to a high electric field in the channel), the transition point between the two regimes has fixed temperature and is independent on the gate bias. However, upon moving to smaller source-drain voltages, this transition point shifts to lower temperatures (higher T-1/2), up to a point where it is not visible anymore. It also becomes more dependent on the gate bias VG (as can be seen especially for VSD = -3 V). Such behaviour has been explained in detail by Bourbie et al.,38-40 who showed that the temperature dependence of DC conductivity in the 1D transport regime is given by equation (7), where T1 is given by (8). Here, (1/α) corresponds to the localization length (that can be changed with VG via Fermi level shift), N is density of states and kB is the Boltzmann constant. The critical temperature Tc, which separates two conductivity regimes, is field dependent and given by (9). Here, e is the electron charge and E is the electric field in the channel (being proportional to VSD).
There also exists the critical electric field EC, corresponding to the energy state
bandwidth Δ as eECR = Δ (with R being the distance between the hopping sites). It puts the limitation on the maximum critical temperature TC(EC) = Δ/2αkBR. 𝜎(𝑇) = 𝜎 𝑒𝑥𝑝 − 𝑇 (𝐸 ) =
Figure 6 presents compiled Tc and slopes of conductivity curves in both regimes. As predicted by equations (7–9), the critical temperature mildly increases with the increased gate bias (and thus localization length). At first sight, there seem to be no VSD dependence, at least at high voltages. This steady behaviour is governed by staying in the regime over the critical electric field. Yet, as soon as the field in the channel drops below the critical value (in our geometry achieved at around 3V), the associated Tc rapidly drops and the transition can no longer be detected by our setup (both due to the very small signals and low temperature).
Figure 6. Critical temperature extracted from Figure 5 plotted as a function of gate bias for different source-drain voltages (A); conductivity slope from Figure 5 in the two regimes – over the Tc (full spots) and below Tc (crossed spots) for varying VG and VSD (B). In the case of T < TC, the tunnelling process (phonon-emission) takes over and T dependence is reduced significantly. Now, the lnσ should be proportional to E-1/2, which is the situation in Figure S10 (Supporting Information). Here we used VSD as it is proportional to E, and only small deviation from linearity is observed at lower gate voltages and/or very low VSD. We also excluded the possibility of transition from a rectangular to triangular energy barrier shape, also known as Fowler-Nordheim tunnelling (FN). Plotting ln(ISD/VSD2) as a function of 1/VSD can give a clear indication on the barrier type.34 Expressions for the rectangular (10) and triangular (11) barriers are given below.
We provide FN plots for the 20 nm C8-BTBT-C8 device obtained for different temperatures in the Supporting Information of Figure S11. In all cases, the curves show logarithmic shapes, indicating a rectangular potential barrier. 21 ACS Paragon Plus Environment
CONCLUSIONS In summary, we investigated a set of symmetrically and asymmetrically alkylated BTBT derivatives and correlated their structural differences to OFET performance. By using different mobility measurement techniques, we observed higher hole mobilities in molecules with symmetric alkylation, assigned to induction of a “zipper effect” which brings sulphur atoms of adjacent BTBT cores in closer proximity. As a result, an increase in intermolecular orbital coupling provides charge transport perpendicular to the plane of the chromophores’ conjugated π-system and along the FET channel. In addition, alkyl chains on both sides of BTBT core prevent core-core stacking, thus creating a more beneficial charge transport pathway. The Gated van der Pauw method was found to be the most reliable technique for measuring FET mobility: It eliminates both impact of the contact resistance and errors coming from geometry dependence of other methods, whilst providing statistical information for a single sample. This method gave very comparable mobility values of 4.2 and 4.3 cm2/Vs for C8-BTBT-C8 and C10BTBT-C10, respectively, and much lower values of 0.4 and 2.7 cm2/Vs for their mono alkylated counterparts. However, it is worth noting that longer (C10) alkyl chains result in reduced film quality. Finally, we applied a compact model of conductivity, including temperature and field based transitions between different conductivity regimes to explain non-Arrhenius temperature dependence of the measured mobility in these materials.
ACKNOWLEDGEMENTS We thank the Australian Research Council (ARC) for financial support (ARC DP140101088 and ARC DP160100700) and Department of Industry, Innovation and Science (AISRF53765) for financial support. E.B.N. is the recipient of a UQ Fellowship. V.A. was funded by an Australian Postgraduate Award. This work was performed in part at the Australian National 22 ACS Paragon Plus Environment
Fabrication Facility Queensland Node (ANFF-Q), a company established under the National Collaborative Research Infrastructure Strategy to provide nano- and microfabrication facilities for Australia’s researchers.
SUPPORTING INFORMATION Material synthesis procedures, photophysical spectroscopy, XRD, AFM, and electrical measurements are provided in the accompanying Supporting Information.
Takimiya, K.; Osaka, I.; Mori, T.; Nakano, M. Organic Semiconductors Based on Benzothieno[3,2-b]Benzothiophene Substructure. Acc. Chem. Res. 2014, 47, 1493–1502. Ullah, M.; Wawrzinek, R.; Maasoumi, F.; Lo, S.-C.; Namdas, E. B. Semitransparent and Low-Voltage Operating Organic Light-Emitting Field-Effect Transistors Processed at Low Temperatures. Adv. Opt. Mater. 2016, 4, 1022–1026. Generali, G.; Soldano, C.; Facchetti, A.; Muccini, M. Innovative Trilayer Organic Light Emitting Transistor (OLET) Structure for Blue Emission. SID Symp. Dig. Tech. Pap. 2016, 47, 1779–1782. Liu, X.; Luo, X.; Nan, H.; Guo, H.; Wang, P.; Zhang, L.; Zhou, M.; Yang, Z.; Shi, Y.; Hu, W.; Ni, Z.; Qiu, T.; Yu, Z.; Xu, J.-B.; Wang, X. Epitaxial Ultrathin Organic Crystals on Graphene for High-Efficiency Phototransistors. Adv. Mater. 2016, 28, 5200–5205. Ullah, M.; Wawrzinek, R.; Maasoumi, F.; Lo, S.-C.; Namdas, E. B. UV–Deep Blue– Visible Light-Emitting Organic Field Effect Transistors with High Charge Carrier Mobilities. Adv. Opt. Mater. 2017, 5, 1600973. Prosa, M.; Benvenuti, E.; Pasini, M.; Giovanella, U.; Bolognesi, M.; Meazza, L.; Galeotti, F.; Muccini, M.; Toffanin, S. Organic Light-Emitting Transistors with Simultaneous Enhancement of Optical Power and External Quantum Efficiency via Conjugated Polar Polymer Interlayers. ACS Appl. Mater. Interfaces 2018, 10, 25580– 25588. Uemura,T.; Rolin, C.; Ke, T. H.; Fesenko, P.; Genoe, J.; Heremans, P.; Takeya, J. On the Extraction of Charge Carrier Mobility in High-Mobility Organic Transistors. Adv. Mater. 2015, 28, 151–155. Bittle, E. G.; Basham, J. I.; Jackson, T. N.; Jurchescu, O. D.; Gundlach, D. J. Mobility Overestimation due to Gated Contacts in organic Field-Effect Transistors. Nat. Commun. 2016, 7, 10908. Liu, C.; Li, G.; Di Pietro, R.; Huang, J.; Noh, Y. Y.; Liu, X.; Minari, T. Device Physics of Contact Issues for the Overestimation and Underestimation of Carrier Mobility in Field-Effect Transistors. Phys. Rev. Appl. 2017, 8, 034020. 23 ACS Paragon Plus Environment
(10) Paterson, A. F.; Singh, S.; Fallon, K. J.; Hodsden, T.; Han, Y.; Schroeder, B. C.; Bronstein, H.; Heeney, M.; McCulloch, I.; Anthopoulos, T. D. Recent Progress in HighMobility Organic Transistors: A Reality Check. Adv. Mater. 2018, 30, 1801079. (11) Miccoli, I.; Edler, F.; Pfnür, H.; Tegenkamp, C. The 100th Anniversary of the Four-Point Probe Technique: the Role of Probe Geometries in Isotropic and Anisotropic Systems. J. Phys. Condens. Matter. 2015, 27, 223201. (12) Anisimov, V. I.; Aryasetiawan, F.; Lichtenstein, A. I. First-Principles Calculations of the Electronic Structure and Spectra of Strongly Correlated Systems: the LDA + U Method. J. Phys. Condens. Matter. 1997, 9, 767–808. (13) Pesavento, P. V.; Puntambekar, K. P.; Frisbie, C. D.; McKeen, J. C.; Ruden, P. P. Tunneling of Anyonic Majorana Excitations in Topological Superconductors. J. Appl. Phys. 2006, 99, 094504. (14) Alkan, M.; Yavuz, I. Intrinsic Charge-Mobility in Benzothieno[3,2-b]benzothiophene (BTBT) Organic Semiconductors is Enhanced with Long Alkyl Side-Chains. Phys. Chem. Chem. Phys. 2018, 20, 15970–15979. (15) Saito, M.; Osaka, I.; Miyazaki, E.; Takimiya, K.; Kuwabara, H.; Ikeda, M. One-Step Synthesis of Benzothieno[3,2-b]Benzothiophene from o-Chlorobenzaldehyde. Tetrahedron Lett. 2011, 52, 285–288. (16) Combe, C. M. S.; Biniek, L.; Schroeder, B. C.; McCulloch, I. Synthesis of Benzothieno[3,2-b]Benzothiophene Pendant and Norbornene Random CoPolymers via Ring Opening Metathesis. J. Mater. Chem. C 2014, 2, 538–541. (17) Inoue, S.; Minemawari, H.; Tsutsumi, J.; Chikamatsu, M.; Yamada, T.; Horiuchi, S.; Tanaka, M.; Kumai, R.; Yoneya, M.; Hasegawa, T. Effects of Substituted Alkyl Chain Length on Solution-Processable Layered Organic Semiconductor Crystals. Chem. Mater. 2015, 27, 3809–3812. (18) Ebata, H.; Izawa, T.; Miyazaki, E.; Takimiya, K.; Ikeda, M.; Kuwabara, H.; Yui, T. Highly Soluble Benzothieno[3,2-b]Benzothiophene (BTBT) Derivatives for HighPerformance, Solution-Processed Organic Field-Effect Transistors. J. Am. Chem. Soc. 2007, 129, 15732–15733. (19) Ruzié, C.; Karpinska, J.; Sanguinet,; A.; Laurent, L.; Hunter, S.; Anthopoulos, T. D.; Lemaur, V.; Cornil, J.; Kennedy, A. R.; Fenwick, O.; Samorì, P.; Schweicher, G.; Chattopadhyay, B.; Geerts, Y. H. Design, Synthesis, Chemical Stability, Packing, Cyclic Voltammetry, Ionisation Potential, and Charge Transport of Benzothieno[3,2b]Benzothiophene Derivatives. J. Mater. Chem. C 2016, 4, 4863–4879. (20) Hunter, C. A.; Sanders, J. K. M. The Nature of - Interactions J. Am. Chem. Soc. 1990, 112, 5525–5534. (21) Vyas, V. S.; Gutzler, R.; Nuss, J.; Kern, K.; Lotsch, B. V. Optical Gap in Herringbone and π-Stacked Crystals of Benzothieno[3,2-b]Benzothiophene and Its Brominated Derivative. CrystEngComm 2014, 16, 7389–7392. (22) Gbabode, G.; Dohr, M.; Balandier, J.; Niebel, C.; Ruzie, C.; Negrier, P.; Mondieig, D.; Geerts, Y. H.; Resel, R.; Sferrazzat, M. X-ray Structural Investigation of Nonsymmetrically and Symmetrically Alkylated Benzothieno[3,2-b]Benzothiophene Derivatives in Bulk and Thin Films. ACS Appl. Mater. Interfaces 2014, 6, 13413–13421. (23) Izawa, T.; Miyazaki, E.; Takimiya, K. Molecular Ordering of High‐Performance Soluble Molecular Semiconductors and Re-evaluation of Their Field-Effect Transistor Characteristics. Adv. Mater. 2008, 20, 3388–3392. 24 ACS Paragon Plus Environment
(24) Inokuchi, H.; Saito, G.; Wu, P.; Seki, K.; Tang, T. B.; Mori, T.; Imaeda, K.; Enoki, T.; Higuchi, Y.; Inaka, K.; Yasuoka, N. A Novel Type of Organic Semiconductors. Molecular Fastener. Chem. Lett. 1986, 1263–1266. (25) Nan, G.; Li, Z. Crystal Structure versus Charge Transport in Organic Single Crystals of Benzothieno[3,2-b]benzothiophene Derivatives from a Multiscale Theoretical Study. J. Mater. Chem. C 2014, 2, 1447–1456. (26) Minemawari, H.; Tsutsumi, J.; Inoue, S.; Yamada, T.; Kumai, R.; Hasegawa, T. Crystal Structure of Asymmetric Organic Semiconductor 7-Decyl-2-phenylBenzothieno[3,2b]Benzothiophene. Appl. Phys. Express 2014, 7, 091601. (27) Marinov, O.; Deen, M. J.; Zschieschang, U.; Klauk, H. Organic Thin-Film Transistors: Part I-Compact DC Modeling. IEEE Trans. Electron Devices 2009, 56, 2952–2961. (28) Marinkovic, M.; Belaineh, D.; Wagner, V.; Knipp, D. On the Origin of Contact Resistances of Organic Thin Film Transistors. Adv. Mater. 2012, 24, 4005–4009. (29) Choi, H. H.; Rodionov, Y. I.; Paterson, A. F.; Panidi, J.; Saranin, D.; Kharlamov, N.; Didenko, S. I.; Anthopoulos, T. D.; Cho, K.; Podzorov, V. Accurate Extraction of Charge Carrier Mobility in 4-Probe Field-Effect Transistors. Adv. Funct. Mater. 2018, 28, 1707105. (30) van der Pauw, L. J. A Method of Measuring the Resistivity and Hall Coefficient on Lamellae of Arbitrary Shape. Philips Tech. Rev. 1958, 20, 220–224. (31) van der Pauw, L. J. A Method of Measuring Specific Resistivity and Hall Effect of Disks of Arbitrary Shape. Philips Res. Rep. 1958, 13, 1–9. (32) Rolin, C.; Kang, E.; Lee, J.-H.; Borghs, G.; Heremans, P.; Genoe, J. Charge carrier Mobility in Thin Films of Organic Semiconductors by the Gated van der Pauw Method. Nat. Commun. 2017, 8, 14975. (33) Dhoot, A. S.; Wang, G. M.; Moses, D.; Heeger, A. J. Voltage-Induced Metal-Insulator Transition in Polythiophene Field-Effect Transistors. Phys. Rev. Lett. 2006, 96, 246403. (34) Dhoot, A. S.; Aramaki, S.; Moses, D.; Heeger, A. J. Metal-Insulator Transition in Solution-Processible Porphyrinic Field-Effect Transistors. Adv. Mater. 2007, 19, 2914– 2917. (35) Kang, E. S. H.; Kim, E. Multi-Barrier Field-Emission Behavior in PBTTT Thin Films at low temperatures. Sci. Rep. 2015, 5, 8396. (36) Yuen, J. D.; Menon, R.; Coates, N. E.; Namdas, E. B.; Cho, S.; Hannahs, S. T.; Moses, D.; Heeger, A. J. Nonlinear Transport in Semiconducting Polymers at High Carrier Densities. Nat. Mater. 2009, 8, 572–575. (37) He, D.; Qiao, J.; Zhang, L.; Wang, J.; Lan, T.; Qian, J.; Li, Y.; Shi, Y.; Chai,Y.; Lan, W.; Ono, L. K.; Qi, Y.; Xu, J. B.; Ji, W.; Wang, X. Ultrahigh Mobility and Efficient Charge Injection in Monolayer Organic Thin-Film Transistors on Boron Nitride. Sci. Adv. 2017, 3, e1701186. (38) Bourbie, D. Field-Induced Crossover from Phonon to Field Assisted Hopping Conductivity in Organic Materials. Appl. Phys. Lett. 2011, 98, 012104. (39) Ikrelef, N.; Bourbie, D.; Driss-Khodja, K. On the Inverse Field Dependence of Conductivity in Disordered Organic Materials. Appl. Phys. Lett. 2010, 97, 022101. (40) Bourbie, D.; Ikrelef, N.; Driss-Khodja, K.; Nedellec, P. Temperature- and FieldDependent Conductivity in Disordered Materials. Phys. Rev. B Condens. Matter Mater. Phys. 2007, 75, 184204. 25 ACS Paragon Plus Environment